LiNa~2~AlF~6~: a powder structure solution
Kirik, Sergei D.; Zaitseva, Julia N.; Yakimov, Igor S.; Golovnev, Nikolay N.; Acta Crystallographica Section C 58 (2002) i159–i160; doi:10.1107/S0108270102018462

data_2013037
_publ_section_title
;
 LiNa~2~AlF~6~: a powder structure solution
;
_journal_issue                   11
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first              i159
_journal_page_last               i160
_journal_paper_doi               10.1107/S0108270102018462
_journal_volume                  58
_journal_year                    2002
_chemical_formula_analytical     'Al F6 Li Na2'
_chemical_formula_iupac          'Li Na2 Al F6'
_chemical_formula_moiety         'Al F6 Li Na2'
_chemical_formula_structural     'Al F6 Li Na2'
_chemical_formula_sum            'Al F6 Li Na2'
_chemical_formula_weight         193.892
_chemical_name_common            'lithium sodium aluminium fluoride'
_chemical_name_systematic
;
lithium disodium aluminium hexafluoride
;
_chemical_temperature_decomposition 1053
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.005(2)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.2863(4)
_cell_length_b                   5.3603(4)
_cell_length_c                   7.5025(6)
_cell_measurement_temperature    293
_cell_volume                     212.59(3)
_computing_cell_refinement       'modified Rietveld program DBWM'
_computing_data_collection       'DRON-4 data collection software'
_computing_data_reduction        'XDIG (local program)'
_computing_molecular_graphics    'XP (Siemens, 19??)'
_computing_structure_refinement  'modified Rietveld program DBWM'
_computing_structure_solution
'Patterson and Fourier synthesis (local program)'
_diffrn_ambient_temperature      295.0(10)
_diffrn_measurement_device_type  'DRON-4 powder diffractometer'
_diffrn_radiation_monochromator  graphite
_refine_ls_goodness_of_fit_all   1.85
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     40
_refine_ls_number_restraints     0
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            iz1026.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

'_chemical_melting_point' tag was changed to
'_chemical_temperature_decomposition' since the value had been
'decomp. 1053 K'. The value 'decomp. 1053 K' was changed to '1053'.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 

The following automatic conversions were performed:

'_chemical_melting_point' tag was changed to
'_chemical_temperature_decomposition' since the value had been
'decomp. 1053 K'. The value 'decomp. 1053 K' was changed to '1053'.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_cell_volume        212.59
_cod_original_sg_symbol_H-M      'P 21/n'
_cod_database_code               2013037